Dramatically increasing the thermal conductivity of silicone rubber composites
April 4, 2017
Author(s): Yonglai Lu
Incorporating small amounts of graphite nanosheets into highly filled spherical-alumina/silicone rubber hybrids strengthens the filler–filler networks.
With the continued miniaturization of electronic device components comes the problem of heat dissipation. This issue means that it is constantly necessary to improve the properties of thermal interface materials (TIMs) in modern chip packaging.1–3 For this reason, elastomeric TIMs are usually fabricated by filling silicone rubber (SiR) with ceramic conductive fillers, i.e., made of alumina (Al2O3), aluminum nitride, boron nitride, or silicon carbide. Of these filler materials, Al2O3 is the most commonly used because of its high performance-to-price ratio. The thermal conductivity of Al2O3/SiR composites, however, is not very high (even with high filler loadings).
A large research effort has thus been dedicated to the use of graphite nanosheets (GNSs) to improve the thermal conductivity of Al2O3/SiR composites.4–10 These materials are excellent heat conductors at room temperature and could thus potentially be used as thermally conducting fillers. Previous studies on the use of GNSs in Al2O3/SiR composites indicate that a high aspect ratio of the dispersed GNSs is an important factor for achieving high thermal conductivity enhancement (TCE) in the nanocomposites. Despite the success of these studies, they involved the use of several mixing techniques and organic solvents (i.e., which are not environmentally friendly). Large-scale fabrication of thermally conductive composites has also been restricted because of the complicated nature of the preparation procedure.
In this work,11 we have therefore developed a more efficient method for the fabrication of thermally conductive SiR composites. In our approach, we use a double planetary mixer—and the direct mechanical compounding method—to achieve nanoscale dispersion of GNSs in liquid SiR. The mixer provides moderate shear forces to ensure good distribution and dispersion of the GNSs, but without severely reducing their aspect ratio. With the use of this solvent-free mixing technique, we are thus able to incorporate small amounts of GNSs (1–5 parts per hundred rubber, phr) into our highly filled S-Al2O3/SiR composites. The spatial distribution of the GNSs and S-Al2O3 in the hybrid filler composites is illustrated schematically in Figure 1. The lateral size of the dispersed GNSs is comparable to the diameter of the S-Al2O3 particles (see Figure 2), which means that the GNSs can act as bridges between the S-Al2O3 particles. Extra networks can also be formed if the distance between the surfaces of neighboring S-Al2O3 particles is less than the lateral size of the GNSs.
Schematic diagram of the spatial distribution of graphite nanosheets (GNSs) and spherical alumina (S-Al2O3) particles in the hybrid silicone rubber (SiR)/S-Al2O3composites at (a) low and (b) high S-Al2O3loadings.
Scanning electron microscope images of fracture surfaces in the SiR/S-Al2O3composites. Images are shown for the (a, b) 100 parts per hundred rubber (phr) S-Al2O3, (c, d) 2phr GNS, (e, f) 100phr S-Al2O3/2phr GNS, and (g, h) 300phr S-Al2O3/2phr GNS samples.
We find that the incorporation of only a small amount of GNSs can dramatically improve the thermal conductivity of both the SiR and the highly filled S-Al2O3/SiR composite samples (see Figure 3). For example, the thermal conductivity of SiR increased from 0.203 to 0.599W/(m·K) after the incorporation of 5 phr of GNSs. This increase corresponds to a TCE of 195%. In addition, we measured an increase in thermal conductivity of the 300phr S-Al2O3/SiR composite from 1.103 to 2.162W/(m·K) upon addition of 5phr GNS (i.e., an improvement of about 96%).
Thermal conductivity of the GNS/SiR and S-Al2O3/GNS/SiR composites as a function of GNS loading.
The strain dependence of the storage modulus (G ′) for filled rubber is generally known as the ‘Payne effect,’ which can be used to qualitatively characterize filler–filler networks. We therefore investigated the Payne effect for our composite samples (with different loadings of S-Al2O3 and GNSs) to indirectly characterize the filler–filler network strength. In particular, we have determined the dynamic storage modulus difference (ΔG ′)—i.e., between the dynamic storage modulus at a very small strain and at a high final strain—which is considered to be a qualitative indication of filler–filler network strength.12 Our results (see Figure 4) show that ΔG ′ (i.e., the filler network strength) of the SiR/S-Al2O3 composites increases with increasing GNS loading (between 0 and 5phr). Furthermore, the change in ΔG ′ with GNS loading varies with S-Al2O3 content. As a result, the filler–filler network is stronger for the 300phr S-Al2O3 sample than for the 100 and 200phr S-Al2O3composites.
Dynamic storage modulus difference (ΔG') for SiR/S-Al2O3composites with GNS loadings of 0–5phr.
We also calculated the thermal conductivity for each of the hybrid filler systems by summing the individual effects of the GNS and S-Al2O3 fillers. In this way, we were able—see Figure 5—to determine the extent of synergy (i.e., the interaction of multiple elements in a system to produce an effect different from, or greater than, the sum of their individual effects) in the composites. We find that the extent of synergy increases with GNS loading and is at the maximum for the 300phr S-Al2O3 composite. We ascribe this synergetic effect to the extra filler–filler networks that are formed by the graphite nanoflakes bridging neighboring S-Al2O3particles. These bridges thus act as an effective pathway for phonon movement in the insulator matrix.13 In addition, our results indicate that the extent of synergy depends on both the composition and loading of the fillers.
Extent of synergy (ϕs) on the thermal conductivity of SiR/S-Al2O3/GNS composites with GNS loadings of 0–5phr.
In summary, we have demonstrated a new and efficient method for producing thermally conductive SiR composites. In this approach, small amounts of GNSs (1–5phr) are added to highly filled S-Al2O3/SiR composites via direct mechanical compounding. Nanoscale dispersion of the GNSs was successfully achieved and the addition of these small GNS loadings produced substantial increases in the thermal conductivity of the samples. The results of the study also indicate that there is a synergetic effect on the thermal conductivity improvement. In our future work, we will try to optimize the blending conditions so that we can further improve the dispersion of the GNSs, and thus reduce their loading.
College of Materials Science and Engineering, Beijing University of Chemical Technology
- P. E. Phelan and R. C. Niemann, Effective thermal conductivity of a thin, randomly oriented composite material, J. Heat Transfer 120, pp. 971-976, 1998.
- J. M. Bustillo, R. T. Howe and R. S. Muller, Surface micromachining for microelectromechanical systems, Proc. IEEE 86, pp. 1552-1574, 2002.
- R. Prasher, Thermal interface materials: historical perspective, status, and future directions, Proc. IEEE 94, pp. 1571-1586, 2006.
- Q. Mu and S. Feng, Thermal conductivity of graphite/silicone rubber prepared by solution intercalation, Thermochim. Acta 462, pp. 70-75, 2007.
- A. Yu, P. Ramesh, M. E. Itkis, E. Bekyarova and R. C. Haddon, Graphite nanoplatelet–epoxy composite thermal interface materials, J. Phys. Chem. C 111, pp. 7565-7569, 2007.
- K. M. F. Shahil and A. A. Balandin, Graphene-multilayer graphene nanocomposites as highly efficient thermal interface materials, Nano Lett. 12, pp. 861-867, 2012.
- M.-T. Hung, O. Choi, Y. S. Ju and H. T. Hahn, Heat conduction in graphite-nanoplatelet-reinforced polymer nanocomposites, Appl. Phys. Lett. 89, pp. 023117, 2006.
- J. Li, M. L. Sham, J.-K. Kim and G. Marom, Morphology and properties of UV/ozone treated graphite nanoplatelet/epoxy nanocomposites, Compos. Sci. Technol. 67, pp. 296-305, 2007.
- J. Tian, I. Miotkowski, S. Hong and Y. P. Chen, Electrical injection and deteciton of spin-polarized currents in topological insulator Bi2Te2Se, Sci. Rep. 5, pp. 14293, 2015.
- K. T. Kim, T. D. Dao, H. M. Jeong, R. V. Anjanapura and T. M. Aminabhavi, Graphene coated with alumina and its utilization as a thermal conductivity enhancer for alumina sphere/thermoplastic polyurethane composite, Mater. Chem. Phys. 153, pp. 291-300, 2015.
- Y. Lu, J. Wang, X. Wang, L. Liu, M. Tian, X. Guan and L. Zhang, Synergetic effect of graphite nanosheets and spherical alumina particles on thermal conductivity enhancement of silicone rubber composites, Polym. Compos., 2016.
- G. Heinrich, M. Klüppel and T. A. Vilgis, Reinforcement of elastomers, Curr. Opin. Solid State Mater. Sci. 6, pp. 195-203, 2002.
- J. Hong, J. Lee, D. Jung and S. E. Shim, Thermal and electrical conduction behavior of alumina and multiwalled carbon nanotube incorporated poly(dimethyl siloxane), Thermochim. Acta 512, pp. 34-39, 2011.